FSC 7530 RECYCLED FORMS BOND, WHITE AND COLORED JCP G15
Bond Paper (50% total recovered material w/30% PC) 1 February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For face only offset and flexographic printing of marginally punched continuous open forms, including multiple copies, principally
on web-type presses. Printed matter may include ruled forms with text, line illustrations, and continuous tones. Slitting and pasting are
included in press capabilities. End use of the paper is generally on impact-type computer printers, and mechanical busters and decollators.
Stock: 100% chemical pulp. Thickness: Average (mm) 0.065 0.070 0.090 0.105 0.115
Note: Not less than 50 pct total recovered fiber of which 30 Equivalent (inch) ............ 0.0026 0.0028 0.0035 0.0041 0.0045
percentage points shall be postconsumer fiber. Recovered fiber, in A tolerance of ±0.013 mm (0.0005 inch) shall be allowed.
any percent over 50 percentage points, is encouraged, provided Paper shall be uniform and shall not vary more than 0.011 mm
that the requirements of this Standard are met.
(0.0004 inch) from one edge to the other.
Grammage (g/m2) ............. 38 45 55 68 75 Ruling and writing qualities: Lines ruled and characters writ-
Basis weight: 17 by 22 ten with ball point and felt tip pens shall be clear cut and free
inches, 500 sheets from excessive feathering.
(pounds) .......................... 10 12 15 18 20 General appearance: Paper shall conform to the standard sam-
A tolerance of ±5 pct shall be allowed. ple(s) adopted by the Government.
Bursting strength: Aver- Color: The paper in the order (or publication) shall be uniform
age, not less than with a target brightness of 77 pct for the white paper. The color
(kPa) ................................ 40 50 60 80 100 variation shall not exceed DE(CIELAB)=1.0.
Equivalent (lb/in2) .......... 6 8 9 12 15 For colored stock, paper shall match one of the established
standards or as specified. Colors shall not fade or transfer (rub
Pick resistance: Average, each side, not less than 10–A Dennison off) and shall appear even and uniform on the surface of the
wax number. sheet. The commercial standard for the color is applicable, un-
No individual specimen shall average less than 8–A Dennison less otherwise specified that the color shall conform to the Gov-
wax number. ernment standard color sample. Stock shall not be 2-sided. Color
Note: Printed forms are used on impact-type computer printers coordinates for selected standards are included in Part 3.
and the above pick values define the degree of resistance to Note: When specifying paper intended for forms which are to
linting and dusting demanded of these forms. be processed on copying machines, tinted paper should not be
Opacity: Average, not used.
less than (percent) .......... 80 80 80 80 80 Finish and formation: Shall be uniform.
No individual specimen Cleanliness: Shall match the Government standard.
shall average less than Sampling and testing: Shall be conducted in accordance with
(percent) .......................... 78 78 78 78 78 standards in Part 2, Government Paper Specification Standards.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Sizing: Paper shall be surface- and internal-sized suitable for sat- Size and trim: Rolls: Roll width and diameter shall be as ordered.
isfactory printing on both sides of the paper on high-speed heat- A tolerance of ±2 mm (1⁄16 inch) shall be allowed for width and
set web offset presses equipped with continuous flow or brush ±26 mm (1 inch) for diameter.
dampening systems. Roll winding: Roll paper shall be tightly wound at even tension
Tensile strength: Average, not less than— and shall not contain more than the specified maximum number
Machine direction of splices per roll. The number of splices permitted per roll is de-
(kN/m) ............................. 1.5 1.6 1.7 1.8 1.9 termined by the roll diameter as ordered. On rolls 1,016 mm (40
Cross direction (kN/m) ... 0.5 0.6 0.7 0.8 0.9 inches) or less, a maximum of three splices per roll shall be al-
Equivalent— lowed. On rolls over 1,016 mm (40 inches), a maximum of four
Machine direction splices per roll shall be allowed. Splices shall be neatly and se-
(kg/in) .............................. 3.9 4.1 4.4 4.6 4.9 curely overlap-pasted and made with a repulpable adhesive
Cross direction (kg/in) .... 1.3 1.6 1.8 2.1 2.3 which will not permit the splice to separate while passing
through a drying oven maintained at 200 °C. The adhesive may
Color: Shall match the Government’s standard sample for color.
A deviation of DE(CIELAB)±3.0 from the color standard for be applied from a tape form backing, provided the backing is re-
white and 2.0 for colored stocks is allowed. A color difference 1.0 moved, leaving only the adhesive component on the splice. The
DE unit between felt and wire sides is permitted. adhesive shall not cause the splice to adhere to adjacent laps.
The tails of the splices shall be neatly and evenly removed with-
Curl: Paper shall lie flat with either no tendency to curl or with out damage to adjacent laps. Splices shall be flagged at both
a curl which can be overcome under reasonable working condi- ends with projecting colored markers, not pasted to the splice,
tions. or otherwise clearly marked.
Surface: Shall be free from lint, fuzz, or any particles which will Pressroom conditions: The bulk of this paper will be used in
pick, lift, fluff, or pile on the blanket under normal press condi- air-conditioned pressrooms maintained at 24 °C ±2 °C and 45 pct
tions. ±8 pct relative humidity.
1 This standard exceeds the EO 13101 minimum content standard.